Presentation on theme: "FHWA BAA Objective 2 Studies - Latifee, Math, Wingard and Rangaraju"— Presentation transcript:
1FHWA BAA Objective 2 Studies - Latifee, Math, Wingard and Rangaraju Investigation of ASR expansion due to total alkali and internal alkali (concentration) in the concreteE. R. Latifee, PhD10th Global Engineering, Science and Technology ConferenceJanuary 2, 2015, BIAM Foundation,63 Eskaton, Dhaka, BangladeshASR TWG Meeting, Albuquerque, NM - December 15-16, 2009
2Acknowledgement Dr. Prasad Rangaraju, Clemson University, U.S.A. Dr. Paul Virmani, FHWA,U.S.A.
3ASR - Alkali Silica Reaction +Reactive SilicaMoistureASR Gel which expandsConcrete expansion andcrackingWhat is Alkali Silica Reaction?Alkali-silica reaction (ASR) is a heterogeneous chemical reaction between alkali ions (Na+ and K+) and hydroxide ions (OH-) in the concrete pore solution, generally derived from the Portland cement, and forms of reactive silica (SiO2) in the aggregate (eg: chert, quartzite, opal, strained quartz crystals).
4Creation of alkali-silica gel and cracking of concrete
5SEM and EDX Analysis of Spratt Specimen scanning electron microscope ImageEnergy-dispersive X-ray spectroscopy
6Alkali-Silica Reaction Distresses in the field FHWA BAA Objective 2 Studies - Latifee, Math, Wingard and RangarajuAlkali-Silica Reaction Distresses in the fieldDeleteASR TWG Meeting, Albuquerque, NM - December 15-16, 2009
9Reference bar and MCPT specimen reading in the comparator
10Storage Condition60 deg. C Storage Room1N NaOH Soak Solution10
11Different Alkali Cements and Soak-solutions- Internal/Pore solution Cement alkali of 0.82% boosted to 1.25% Na2Oeq and 1 N NaOHCement soak solution matching pore solutionCement alkali of 0.82% Na2Oeq and 0.7 N NaOH soak solution matching pore solutionCement alkali of 0.49% Na2Oeq and 0.45 N NaOH soak solution matching pore solution The pore solution composition of the concrete mixtures was predicted based on the equation[OH-] = Na2Oeq%/(w/c) /- 0.06 mol/L-Stark and Diamond (1993)
12Expansion curves of different cement alkalinity and soak solution alkalinity concrete prisms in the MCPT
13Figure: 28-day % expansion vs. Soak solution alkalinity
14Alkali loading of different MCPT specimens Alkali loading, kg/m3 (lb/yd3) = Cement content, kg/m3 (lb/yd3) x Cement Alkalinity (Na2Oeq %).
15Alkali loading and corresponding 56-day expansions of MCPT specimens
16Comparison between alkali loading(lb/yd3) & 56-day % expansion
17Comparison between alkali loading(kg/m3) & 56-day % expansion
18Implementation of MCPT Method and AASHTO Code Round Robin Testing of MCPT -conducted across six labs:Nebraska DOT( Department of Transportation)Delaware DOTTurner-Fairbanks Highway Research Center, FHWAPurdue UniversityBowser Morner, Inc.Clemson UniversityAASHTO adopted Miniature Concrete Prism Test as a provisional test standard AASHTO TP 111 in 2014.Questions?